Electromagnetic modeling of waveguide amplifier based on Nd^{3+} Si-rich SiO_{2} layers by means of the ADE-FDTD method
- Christian Dufour^{1}Email author,
- Julien Cardin^{1},
- Olivier Debieu^{1},
- Alexandre Fafin^{1} and
- Fabrice Gourbilleau^{1}
DOI: 10.1186/1556-276X-6-278
© Dufour et al; licensee Springer. 2011
Received: 27 September 2010
Accepted: 4 April 2011
Published: 4 April 2011
Abstract
By means of ADE-FDTD method, this paper investigates the electromagnetic modelling of a rib-loaded waveguide composed of a Nd^{3+} doped Silicon Rich Silicon Oxide active layer sandwiched between a SiO_{2} bottom cladding and a SiO_{2} rib. The Auxilliary Differential Equations are the rate equations which govern the levels populations. The Finite Difference Time Domain (FDTD) scheme is used to solve the space and time dependent Maxwell equations which describe the electromagnetic field in a copropagating scheme of both pumping (λ _{ pump } = 488 nm) and signal (λ _{ signal } = 1064 nm) waves. Such systems are characterized by extremely different specific times such as the period of electromagnetic field ~ 10^{-15} s and the lifetimes of the electronic levels between ~ 10^{-10}s and ~ 10^{-4} s. The time scaling method is used in addition to specific initial conditions in order to decrease the computational time. We show maps of the Poynting vector along the propagation direction as a function of the silicon nanograin (Si-ng) concentrations. A threshold value of 10^{24} Si-ng m^{-3} is extracted below which the pump wave can propagate so that a signal amplication is possible.
Keywords
Silicon nanograin Silica Neodymium ADE-FDTD Waveguide amplificationIntroduction
The feasibility of optical amplifying waveguide has been for almost two decades the purpose of numerous experimental works [1]. The devices under study were based on an active layer constituted of a silica film co-doped with silicon nanograins (Si-ng) and rare earth ions RE (Er^{3+} in particular) deposited on a substrate and covered by a cladding layer of pure silica. The differences in the optical indices of the three layers ensure the optical guiding. The amplification of a signal is based on an efficient population inversion of the rare earth levels whose energy difference correspond to the signal wavelength. Due to the very low RE signal absorption cross section, a solution has been found using silicon nanoparticles. The physical background lies on two major phenomena: on the one hand, the ability of Si-ng's to absorb efficiently a pumping light and, on the other hand, the effective energy transfer between Si-ng's and RE ions. In this way, a RE population inversion could have been achieved in order to fulfill the amplification function of the device. Despite all these promising features, a net gain is hardly achievable with the former Er^{3+} ions due to their great probability of signal reabsorption from the ground state. This drawback is prevented with the use of Nd^{3+} ions described by a five level scheme since the transition does not involve the ground state. The theoretical studies of the waveguide amplifiers have accounted for both rate population equations and Maxwell equations. In this paper we investigate the ADE-FDTD method applied to a rib-loaded waveguide whose active layer is composed of a silica film co doped with Nd^{3+} ions and silicon nanograins. One of the main issues to be addressed in such systems consists in dealing with extremely different time scales: the populations lifetimes (1 ms) and the electromagnetic field period (10^{-15} s). According to [2, 3] we use a time scaling that allows to circumvent this issue. All the lifetimes have been shortened by a factor of 10^{6}, and consequently the transfer coefficient K has also been divided by the same coefficient. In this paper, we investigate the accuracy of this scaling method through longitudinal and trans-verse maps of the Poynting vector for several Si-ng concentrations. The applicability of this method is linked to the space and time calculation steps since a reasonable computing time must not be exceeded.
Computational details
Four zones appear and will be described hereafter: i) the rib-loaded waveguide composed of the active layer (optical index n _{ act } = 1.52) stacked between the SiO_{2} cladding and rib (optical index ), ii) the plane containing the electromagnetic field source (z _{ source } = 6 Δz), iii) the diaphragm (between 7Δz and 10Δz) which transforms the source into a realistic electromagnetic Gaussian field impinging on the waveguide and iv) the boundary zone (PML) (4Δz in thickness) characterized by appropriate values of electrical (ρ) and magnetic (σ) conductivities in order to absorb the electromagnetic field so that the box borders do not influence the field in the zone of interest [4].
Lorentz Model for the dielectric susceptibility
Δω _{ ij } is the FWHM of the ij transition deduced from photoluminescence measurements according to [5], is the oscillator pulsation linked to the ij transition wavelengh λ _{ ij } , and γ _{ ij } is the ij radiative transition rate in s^{-1}[6, 7]. The level populations difference in m^{-3} is given by ΔN _{ ij } = N _{ i } - N _{ j } .
In the same way, we describe the polarisation density P _{ si } linked to the silicon level populations N _{ Si } (ground level) and (excited level),to the oscillator pulsation ω _{ Si } and finally to the transition FWHM Δω _{ Si } .
Maxwell equations: FDTD numerical method
All the calculations are performed with real variables. Hence, in order to account for absorption processes other than those due to the level transitions, we characterize (especially for the diaphragm and PML) a specific electric conductivity σ and magnetic conductivity ρ.
Both equations 2 and 3 are solved using the Yee algorithm[8]. The space steps are chosen so that: Δx = Δy = Δz ≪ λ _{ min } (the lowest values among all the wavelengths) Hereafter: Δx = Δy = Δz = 45 nm. The time step Δt must fulfill the condition: . Finally the fields inputs (pump and signal) are known as the 'source issue'. Since no perfect source is available, we choose an xy plane at z _{ source } = 6Δz in which we define a polarized electric field. . This source impinges on the diaphragm so that a Gaussian beam enters the waveguide itself at z = 11 Δz. The total waveguide length is 15Δz = 0.665 μ m and the number of time steps is 25000, which amounts to a total simulated time of 0.3 10^{-12} s.
Rate equations
In this section, we detail the ADE part of the method which describes the time population dynamics of Si-ng and Nd^{3}+ levels with the following rate equations.
Silicon nanoclusters
Rare earth ions Nd ^{3+}
We consider three radiative transitions (4F _{3/2} → 4I _{9/2}, λ _{20} = 945 nm; 4F _{3/2} →4I _{11/2}, λ _{21} = 1064 nm; and 4F _{3/2} → 4I _{13/2}, λ _{24} = 1340 nm) and three non radiative transitions (4F _{5/2} - > 4F _{3/2} (N _{3} ↦ N _{2} ) 4I _{11/2} - > 4I _{9/2} (N _{1} ↦ N _{ 0 } ) and 4I _{13/2} - > 4I _{11/2} (N _{4} ↦ N _{1})).
The terms , and correspond to the stimulated transitions 2 → 1, 2 → 0 and 2 → 4. The terms , and correspond to the spontaneous transitions 2 → 1, 2 → 0 and 2 → 4.
Application to rib-loaded waveguide
Simulation parameters of the Si-ng and Nd^{3+} transitions.
Transition | lifetime(s) | type | ω _{ ij }(s ^{-1}) | Δω _{ ij }(s ^{-1}) |
---|---|---|---|---|
Si →Si * | 4 10^{-11} | R | 3.86 10^{15} | 4.4 10^{14} |
3 → 2 | 2.3 10^{-16} | NR | ||
2 → 0 | 3 10^{-10} | R | 2.07 10^{15} | 1.38 10^{14} |
2 → 1 | 3 10^{-10} | R | 1.7 10^{15} | 1.39 10^{14} |
2 → 4 | 3 10^{-10} | R | 1.3 10^{15} | 1.33 10^{14} |
4 → 1 | 9.7 10^{-16} | NR | ||
1 → 0 | 5.1 10^{-16} | NR |
The transfer coefficient K estimated to ~ 10^{-20} m^{3} s^{-1}[11] has also been scaled with the same factor 10^{6}: K = 10^{-14} m^{3}.s^{-1}. The amplitudes of the input pumping and signal electric fields have been taken equal to E _{ pump } = 10^{7} V.m^{-1} and E _{ signal } = 100 V.m^{-1}.
After the time Fourier transform of both E and H fields, we deduce the z component of the pump ( ) and signal ( ) Poynting vectors (in W.m.^{-2})
In these figures, the different calculation box zones may be recognized: i) the Perfectly Matched Layer (PML) which lies in the area from the lefthand side between z = 0 nm and z = 180 nm, and from the righthand side between z = 890 nm and z = 1000 nm, ii) the plane containing the electromagnetic field source at z ~ 300 nm, iii) the FDTD zone which is located at about 180 nm from border of plot, the Gaussian beam impinging in the waveguide at z ~ 500 nm and the intensity propagating in waveguide from z ~ 500 nm to z ~ 900 nm.
On the basis of the parameters taken from experiments, these plots evidence the fact that for Si-ng concentrations above 10^{24} m^{-3}, the pumping wave does not reach the end of the waveguide. This concentration threshold corresponds to high experimental values [12], and is above the lower values leading to minimal optical losses [1].
Conclusion
We have investigated by means of ADE-FDTD method the electromagnetic field propagation in rib-loaded waveguides constituted of an active layer of Nd^{3+} doped silicon rich silica stacked between pure silica bottom cladding and rib. This numerical method treats Nd^{3+} and Si-ng levels rate equations (ADE) coupled to the Maxwell equations (FDTD). The extremely different specific times involved in the ADE (levels lifetimes ≈ 10 μ s) and in FDTD (electromagnetic wave periods ≈ 10^{-15} s) have required the use of the scaling time method which allows reasonable computing time: the number of time iterations has been reduced by six orders of magnitude. In addition to this method, we have proposed to start the calculations with steady state Si-ng ground and excited populations. The numerical computation has been performed for several Si-ng concentrations. Therefore we can infer that the pumping wave propagation (λ _{ pump } = 488 nm ) is possible for [Si-ng] ≤ 10^{24} m^{-3} in agreement with experimental loss measurements. The upper Nd^{3+} level reaches its stationary value predicted with the analytical solution of the steady state rate equations.
Declarations
Acknowledgements
The authors are grateful to the French Agence Nationale de la Recherche, which supported this work through the Nanoscience and Nanotechnology program (DAPHNES project ANR-08-NANO-005).
Authors’ Affiliations
References
- Navarro-Urrios D, Melchiorri M, Daldosso N, Pavesi L, García C, Pellegrino P, Garrido B, Pucker G, Gourbilleau F, Rizk R: Optical losses and gain in silicon-rich Silica waveguides containing Er ions. Journal of Luminescence 2006, 121: 249–255. 10.1016/j.jlumin.2006.08.002View ArticleGoogle Scholar
- Shi S, Prather DW: Lasing dynamics of a silicon photonic crystal microcavity. Opt Express 2007, 15(16):10294–10302. 10.1364/OE.15.010294View ArticleGoogle Scholar
- Redding B, Shi S, Creazzo T, Prather DW: Electromagnetic modeling of active silicon nanocrystal waveguides. Opt Express 2008, 16: 8792–8799. 10.1364/OE.16.008792View ArticleGoogle Scholar
- Berenger JP: A perfectly matched layer for the absorption of electromagnetic waves. J of Computational Physics 1994, 114(2):185–200. 10.1006/jcph.1994.1159View ArticleGoogle Scholar
- Biallo D, De Sario M, Petruzzelli V, Prudenzano F: Time domain analysis of optical amplification in Er3+ doped SiO2-TiO2 planar waveguide. Opt Express 2005, 13(12):4683–4692. 10.1364/OPEX.13.004683View ArticleGoogle Scholar
- Taflove A, Hagness SC, et al.: Computational electrodynamics: the finite-difference time-domain method. Artech House Norwood, MA 1995.Google Scholar
- Zhukovsky SV, Chigrin DN: Numerical modelling of lasing in microstructures. Phys Status Solidi (b) 2007, 244(10):3515–3527. 10.1002/pssb.200743188View ArticleGoogle Scholar
- Yee K: Numerical solution of inital boundary value problems involving Maxwell's equations in isotropic media IEEE Transactions on antennas and propagation. 1966, 14(3):302–307.Google Scholar
- Serqueira EO, Dantas NO, Monte AFG, Bell MJV: Judd Ofelt calculation of quantum efficiencies and branching ratios of Nd3+ doped glasses. J of Non-Crystalline Solids 2006, 352(32–35):3628–3632. 10.1016/j.jnoncrysol.2006.03.093View ArticleGoogle Scholar
- Pecoraro E, Sampaio JA, Nunes LAO, Gama S, Baesso ML: Spectroscopic properties of water free Nd2O3-doped low silica calcium aluminosilicate glasses. J of Non-Crystalline Solids 2000, 277(2–3):73–81. 10.1016/S0022-3093(00)00316-1View ArticleGoogle Scholar
- Pacifici Domenico, Franzò Giorgia, Priolo Francesco, Iacona Fabio, Dal Negro Luca: Modeling and perspectives of the Si nanocrystals-Er interaction for optical amplification. Phys Rev B 2003, 67(24):245301. 10.1103/PhysRevB.67.245301View ArticleGoogle Scholar
- Gourbilleau F, Levalois M, Dufour C, Vicens J, Rizk R: Optimized conditions for an enhanced coupling rate between Er ions and Si nanoclusters for an improved 1.54-μm emission. J Appl Phys 2004, 95: 3717. 10.1063/1.1655680View ArticleGoogle Scholar
Copyright
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.